Boron nitride Identifiers CAS number PubChem ChemSpider EC number MeSH ChEBI RTECS number ED7800000 Gmelin Reference 216 Jmol-3D images Image 1 Properties Molecular formula BN Molar mass 24.82 g mol−1 Exact mass 25.012379471 g mol−1 Appearance Colorless crystals Density 2.1 (hBN); 3.45 (cBN) g cm−3 Melting point
2973 °C, 3246 K, 5383 °F (sublimes (cBN))
Electron mobility 200 cm2/(V·s) (cBN) Refractive index (nD) 1.8 (hBN); 2.1 (cBN) Structure Crystal structure hexagonal, sphalerite, wurtzite Thermochemistry Std enthalpy of
o298 -250.91 kJ mol−1 Standard molar
o298 14.77 J K−1 mol−1 Hazards EU classification Xi R-phrases S-phrases , NFPA 704 Related compounds Related compounds Boron arsenide
(what is: /?)
Except where noted otherwise, data are given for materials in their standard state (at 25 °C, 100 kPa)
Boron nitride is a chemical compound with chemical formula BN, consisting of equal numbers of boron and nitrogen atoms. BN is isoelectronic to a similarly structured carbon lattice and thus exists in various crystalline forms. The hexagonal form corresponding to graphite is the most stable and softest among BN polymorphs, and is therefore used as a lubricant and an additive to cosmetic products. The cubic (sphalerite structure) variety analogous to diamond is called c-BN. Its hardness is inferior only to diamond, but its thermal and chemical stability is superior. The rare wurtzite BN modification is similar to lonsdaleite and may even be harder than the cubic form.
Boron nitride is not found in nature and is therefore produced synthetically from boric acid or boron trioxide. The initial product is amorphous BN powder, which is converted to crystalline h-BN by heating in nitrogen flow at temperatures above 1500 °C. c-BN is made by annealing h-BN powder at higher temperatures, under pressures above 5 GPa. Contrary to diamond, larger c-BN pellets can be produced by fusing (sintering) relatively cheap c-BN powders. As a result, c-BN is widely used in mechanical applications.
Because of excellent thermal and chemical stability, boron nitride ceramics are traditionally used as parts of high-temperature equipment. Boron nitride has a great potential in nanotechnology. Nanotubes of BN can be produced that have a structure similar to that of carbon nanotubes, i.e. graphene (or BN) sheets rolled on themselves, however the properties are very different: whereas carbon nanotubes can be metallic or semiconducting depending on the rolling direction and radius, a BN nanotube is an electrical insulator with a wide bandgap of ~5.5 eV (same as in diamond), which is almost independent of tube chirality and morphology. Similar to other BN forms, BN nanotubes are more thermally and chemically stable than carbon nanotubes which favors them for some applications.
- 1 Structure
- 2 Properties
- 3 Synthesis
- 4 Applications
- 5 Other BN forms
- 6 Health issues
- 7 See also
- 8 Notes and references
- 9 External links
Boron nitride has been produced in an amorphous (a-BN) and crystalline forms. The most stable crystalline form is the hexagonal one, also called h-BN, α-BN, or g-BN (graphitic BN). It has a layered structure similar to graphite. Within each layer, boron and nitrogen atoms are bound by strong covalent bonds, whereas the layers are held together by weak van der Waals forces. The interlayer "registry" of these sheets differs, however, from the pattern seen for graphite, because the atoms are eclipsed, with boron atoms lying over and above nitrogen atoms. This registry reflects the polarity of the B-N bonds. Still, h-BN and graphite are very close neighbors and even the BC6N hybrids have been synthesized where carbon substitutes for some B and N atoms.
As diamond is less stable than graphite, cubic BN is less stable than h-BN, but the conversion rate between those forms is negligible at room temperature. The cubic form has the sphalerite crystal structure, same as diamond structure, and is also called β-BN or c-BN. The wurtzite BN form (w-BN) has similar structure as lonsdaleite, rare hexagonal polymorph of carbon. In both c-BN and w-BN boron and nitrogen atoms are grouped into tetrahedra, but the angles between neighboring tetrahedra are different.
α-BN, hexagonal β-BN, sphalerite structure BN, wurtzite structure
Properties of amorphous and crystalline BN, graphite and diamond.
Some properties of h-BN and graphite differ within the basal planes (║) and perpendicular to them (╧)
Material a-BN h-BN c-BN w-BN graphite diamond Density (g/cm3) 2.28 ~2.1 3.45 3.49 ~2.1 3.515 Mohs hardness 1–2 ~10 ~10 1–2 10 Knoop hardness (GPa) 10 45 34 100 Bulk modulus (GPa) 100 36.5 400 400 34 440 Thermal conductivity (W/cm K) 0.03 6║; 0.3 ┴ 7.4 2–20║; 0.02–0.8┴ 6–20 Thermal expansion (10−6/°C) −2.7║; 38┴ 1.2 2.7 −1.5║; 25┴ 0.8 Bandgap (eV) 5.05 5.2 6.4 4.5–5.5 0 5.5 Refractive index 1.7 1.8 2.1 2.05 2.4 Magnetic susceptibility (µemu/g) −0.48║; -17.3┴ −0.2..-2.7║; -20..-28┴ −1.6
The partly ionic structure of BN layers in h-BN reduces covalency and electrical conductivity, whereas the interlayer interaction increases resulting in higher hardness of h-BN relative to graphite. The reduced electron-delocalization in hexagonal-BN is also indicated by its absence of color and a large band gap. Very different bonding – strong covalent within the basal planes (planes where boron and nitrogen atoms are covalently bonded) and weak between them – causes high anisotropy of most properties of h-BN.
For example, the hardness, electrical and thermal conductivity are much higher within the planes than perpendicular to them. On the contrary, the properties of c-BN and w-BN are more homogeneous.
Those materials are extremely hard, with the hardness of c-BN being slightly smaller and w-BN even higher than that of diamond. Because of much better stability to heat and metals, c-BN surpasses diamond in mechanical applications. The thermal conductivity of BN is among the highest of all electric insulators (see table).
Boron nitride can be doped p-type with Be and n-type with boron, sulfur, silicon or if co-doped with carbon and nitrogen. Both hexagonal and cubic BN are wide-gap semiconductors with a band gap energy corresponding to the UV region. If voltage is applied to h-BN  or c-BN, then it emits UV light in the range 215–250 nm and therefore can potentially be used as light emitting diodes (LEDs) or lasers.
Hexagonal and cubic (and probably w-BN) BN show remarkable chemical and thermal stabilities. For example, h-BN is stable to decomposition in temperatures up to 1000 °C in air, 1400 °C in vacuum, and 2800 °C in an inert atmosphere. The reactivity of h-BN and c-BN is relatively similar, and the data for c-BN are summarized in the table below.
Reactivity of c-BN with solids Solid Ambient Action Threshold T (°C) Mo 10−2 Pa vacuum reaction 1360 Ni 10−2 Pa vacuum wetting 1360 Fe, Ni, Co argon react 1400–1500 Al 10−2 Pa vacuum wetting and reaction 1050 Si 10−3 Pa vacuum wetting 1500 Cu, Ag, Au, Ga, In, Ge, Sn 10−3 Pa vacuum no wetting 1100 B no wetting 2200 Al2O3 + B2O3 10−2 Pa vacuum no reaction 1360
Thermal stability of c-BN can be summarized as follows:
- In air or oxygen: B2O3 protective layer prevents further oxidation to ~1300 °C; no conversion to hexagonal form at 1400 °C.
- In nitrogen: some conversion to h-BN at 1525 °C after 12 h.
- In vacuum (10−5 Pa): conversion to h-BN at 1550–1600 °C.
Boron nitride is insoluble in usual acids, but is soluble in alkaline molten salts and nitrides, such as LiOH, KOH, NaOH-Na2CO3, NaNO3, Li3N, Mg3N2, Sr3N2, Ba3N2 or Li3BN2, which are therefore used to etch BN.
The theoretical thermal conductivity of hexagonal Boron nitride nanoribbons (BNNRs) can approach 1700–2000 W/(m·K), which has the same order of magnitude as the experimental measured value for graphene, and can be comparable to the theoretical calculations for graphene nanoribbons. Moreover, the thermal transport in the BNNRs is anisotropic. The thermal conductivity of zigzag-edged BNNRs is about 20% larger than that of armchair-edged nanoribbons at room temperature.
Boron nitride has not been found in nature and therefore is produced synthetically. The most common raw materials for BN synthesis, boric acid and boron trioxide are produced on industrial scales by treating minerals borax and colemanite with sulfuric acid or hydrochloric acid:
- Na2B4O7·10H2O (borax) + H2SO4 → 4 H3BO3 (boric acid) + Na2SO4 + 5 H2O
Boron trioxide is obtained by heating boric acid.
Preparation and reactivity of hexagonal BN
- B2O3 + 2 NH3 → 2 BN + 3 H2O (T = 900 °C)
- B(OH)3 + NH3 → BN + 3 H2O (T = 900 °C)
- B2O3 + CO(NH2)2 → 2 BN + CO2 + 2 H2O (T > 1000 °C)
- B2O3 + 3 CaB6 + 10 N2 → 20 BN + 3 CaO (T > 1500 °C)
The resulting disordered (amorphous) boron nitride contains 92–95% BN and 5–8% B2O3. The remaining B2O3 can be evaporated in a second step at temperatures >1500 °C in order to achieve BN concentration >98%. Such annealing also crystallizes BN, the size of the crystallites increasing with the annealing temperature.
h-BN parts can be fabricated inexpensively by hot-pressing with subsequent machining. The parts are made from boron nitride powders adding boron oxide for better compressibility. Thin films of boron nitride can be obtained by chemical vapor deposition from boron trichloride and nitrogen precursors. Combustion of boron powder in nitrogen plasma at 5500 °C yields ultrafine boron nitride used for lubricants and toners.
Intercalation of hexagonal BN
Similar to graphite, various molecules, such as NH3 or alkali metals, can be intercalated into hexagonal boron nitride, that is inserted between its layers. Both experiment and theory suggest the intercalation is much more difficult for BN than for graphite.
Preparation of cubic BN
Synthesis of c-BN uses same methods as that of diamond: Cubic boron nitride is produced by treating hexagonal boron nitride at high pressure and temperature, much as synthetic diamond is produced from graphite. Direct conversion of hexagonal boron nitride to the cubic form has been observed at pressures between 5 and 18 GPa and temperatures between 1730 and 3230 °C, that is similar parameters as for direct graphite-diamond conversion. The addition of a small amount of boron oxide can lower the required pressure to 4–7 GPa and temperature to 1500 °C. As in diamond synthesis, to further reduce the conversion pressures and temperatures, a catalyst is added, such as lithium, potassium, or magnesium, their nitrides, their fluoronitrides, water with ammonium compounds, or hydrazine. Other industrial synthesis methods, again borrowed from diamond growth, use crystal growth in a temperature gradient, or explosive shock wave. The shock wave method is used to produce material called heterodiamond, a superhard compound of boron, carbon, and nitrogen.
Low-pressure deposition of thin films of cubic boron nitride is possible. As in diamond growth, the major problem is to suppress the growth of hexagonal phases (h-BN or graphite, respectively). Whereas in diamond growth this is achieved by adding hydrogen gas, boron trifluoride is used for c-BN. Ion beam deposition, plasma-enhanced chemical vapor deposition, pulsed laser deposition, reactive sputtering, and other physical vapor deposition methods are used as well.
Preparation of wurtzite BN
Wurtzite BN can be obtained via static high-pressure or dynamic shock methods. The limits of its stability are not well defined. Both c-BN and w-BN are formed by compressing h-BN, but formation of w-BN occurs at much lower temperatures close to 1700 °C.
Whereas the production and consumption figures for the raw materials used for BN synthesis, namely boric acid and boron trioxide, are well known (see boron), the corresponding numbers for the boron nitride are not listed in statistical reports. An estimate for the 1999 world production is 300 to 350 metric tons. The major producers and consumers of BN are located in the United States, Japan, China and Germany. In 2000, prices varied from about $75/kg to $120/kg for standard industrial-quality h-BN and were about up to $200–$400/kg for high purity BN grades.
Hexagonal BN is the most widely used polymorph. It is a good lubricant at both low and high temperatures (up to 900 °C, even in an oxidizing atmosphere). h-BN lubricant is particularly useful when the electrical conductivity or chemical reactivity of graphite (alternative lubricant) would be problematic. Another advantage of h-BN over graphite is that its lubricity does not require water or gas molecules trapped between the layers. Therefore, h-BN lubricants can be used even in vacuum, e.g. in space applications. The lubricating properties of fine-grained h-BN are used in cosmetics, paints, dental cements, and pencil leads.
Hexagonal BN was first used in cosmetics around 1940 in Japan. However, because of its high price, h-BN was soon abandoned for this application. Its use was revitalized in the late 1990s with the optimization h-BN production processes, and currently h-BN is used by nearly all leading producers of cosmetic products for foundations, make-up, eye shadows, blushers, kohl pencils, lipsticks and other skincare products.
Because of its excellent thermal and chemical stability, boron nitride ceramics are traditionally used as parts of high-temperature equipment. h-BN can be included in ceramics, alloys, resins, plastics, rubbers, and other materials, giving them self-lubricating properties. Such materials are suitable for construction of e.g. bearings and in steelmaking. Plastics filled with BN have less thermal expansion as well as higher thermal conductivity and electrical resistivity. Due to its excellent dielectric and thermal properties, BN is used in electronics e.g. as a substrate for semiconductors, microwave-transparent windows, and as a structural material for seals.
Hexagonal BN is used in xerographic process and laser printers as a charge leakage barrier layer of the photo drum. In the automotive industry, h-BN mixed with a binder (boron oxide) is used for sealing oxygen sensors, which provide feedback for adjusting fuel flow. The binder utilizes the unique temperature stability and insulating properties of h-BN.
Parts can be made of h-BN by hot pressing. Union Carbide Corporation produces three grades of BN. HBN, with boron oxide binder, usable to 550–850 °C in oxidizing atmosphere and up to 1600 °C in vacuum, but due to the boron oxide content is sensitive to water. HBR uses calcium borate binder and is usable at 1600 °C. HBC grade uses no binder and can be used to 3000 °C.
Cubic boron nitride
Cubic boron nitride (CBN or c-BN) is widely used as an abrasive. Its usefulness arises from its insolubility in iron, nickel, and related alloys at high temperatures, whereas diamond is soluble in these metals to give carbides. Polycrystalline c-BN (PCBN) abrasives are therefore used for machining steel, whereas diamond abrasives are preferred for aluminum alloys, ceramics, and stone. When in contact with oxygen at high temperatures, BN forms a passivation layer of boron oxide. Boron nitride binds well with metals, due to formation of interlayers of metal borides or nitrides. Materials with cubic boron nitride crystals are often used in the tool bits of cutting tools. For grinding applications, softer binders, e.g. resin, porous ceramics, and soft metals, are used. Ceramic binders can be used as well. Commercial products are known under names "Borazon" (by Diamond Innovations), and "Elbor" or "Cubonite" (by Russian vendors). Similar to diamond, the combination in c-BN of highest thermal conductivity and electrical resistivity is ideal for heat spreaders. Contrary to diamond, large c-BN pellets can be produced in a simple process (called sintering) of annealing c-BN powders in nitrogen flow at temperatures slightly below the BN decomposition temperature. This ability of c-BN and h-BN powders to fuse allows cheap production of large BN parts.
As cubic boron nitride consists of light atoms and is very robust chemically and mechanically, it is one of the popular materials for X-ray membranes: low mass results in small X-ray absorption, and good mechanical properties allow usage of thin membranes, thus further reducing the absorption.
Amorphous boron nitride
Layers of amorphous boron nitride (a-BN) are used in some semiconductor devices, e.g. MISFETs. They can be prepared by chemical decomposition of trichloroborazine with caesium, or by thermal chemical vapor deposition methods. Thermal CVD can be also used for deposition of h-BN layers, or at high temperatures, c-BN.
Other BN forms
Boron nitride fibers
Hexagonal BN can be prepared in the form of fibers, structurally similar to carbon fibers, by thermal decomposition of extruded borazine (B3N3H6) fibers with addition of boron oxide in a nitrogen atmosphere at 1800 °C. An alternative method is thermal decomposition of cellulose fibers impregnated with boric acid or ammonium tetraborate in an atmosphere of ammonia and nitrogen above 1000 °C. Boron nitride fibers are used as reinforcement in composite materials, with the matrix materials ranging from organic resins to ceramics to metals (see Metal matrix composites).
Boron nitride nanomesh
Boron nitride nanomesh is an inorganic nanostructured two-dimensional material. It consists of a single BN layer, which forms by self-assembly a highly regular mesh after high-temperature exposure of a clean rhodium or ruthenium surface to borazine under ultra-high vacuum. The nanomesh looks like an assembly of hexagonal pores. The distance between 2 pore centers is 3.2 nm and the pore diameter is ~2 nm.
The boron nitride nanomesh is not only stable to decomposition under vacuum, air and some liquids, but also up to temperatures of 800 °C. In addition, it shows the extraordinary ability to trap molecules and metallic clusters which have similar sizes to the nanomesh pores, forming a well-ordered array. These characteristics promise interesting applications of the nanomesh in areas like nanocatalysis, surface functionalisation, spintronics, quantum computing and data storage media like hard drives.
Boron nitride nanotubes
Boron nitride nanotubes were theoretically predicted in 1994 and experimentally discovered in 1995. They can be imagined as a rolled up sheet of boron nitride. Structurally, it is a close analog of the carbon nanotube, namely a long cylinder with diameter of several to hundred nanometers and length of many micrometers, except carbon atoms are alternately substituted by nitrogen and boron atoms. However, the properties of BN nanotubes are very different: whereas carbon nanotubes can be metallic or semiconducting depending on the rolling direction and radius, a BN nanotube is an electrical insulator with a bandgap of ~5.5 eV, basically independent of tube chirality and morphology. In addition, a layered BN structure is much more thermally and chemically stable than a graphitic carbon structure.
All well-established techniques of carbon nanotube growth, such as arc-discharge, laser ablation and chemical vapor deposition, are used to synthesize BN nanotubes. BN nanotubes can also be produced by ball milling of amorphous boron, mixed with a catalyst: iron powder, under NH3 atmosphere. Subsequent annealing at ~1100 °C in nitrogen flow transforms most of the product into BN.
Electrical and field emission properties of the thus prepared nanotubes can be tuned by doping with gold atoms via sputtering of gold on the nanotubes. Doping rare-earth atoms of europium turns a BN nanotube into a phosphor material emitting visible light under electron excitation.
Like BN fibers, boron nitride nanotubes show promise for aerospace applications where integration of boron and in particular the light isotope of boron (10B) into structural materials improves their radiation-shielding properties; the improvement is due to strong neutron absorption by 10B. Such 10BN materials are of particular theoretical value as composite structural materials in future manned interplanetary spacecraft, where absorption-shielding from cosmic ray spallation neutrons is expected to be a particular asset in light construction materials.
Composites containing BN
Addition of boron nitride to silicon nitride ceramics improves the thermal shock resistance of the resulting material. For the same purpose, BN is added also to silicon nitride-alumina and titanium nitride-alumina ceramics. Other materials being reinforced with BN are, e.g., alumina and zirconia, borosilicate glasses, glass ceramics, enamels, and composite ceramics with titanium boride-boron nitride and titanium boride-aluminium nitride-boron nitride and silicon carbide-boron nitride composition.
Boron nitride (along with Si3N4, NbN, and BNC) is reported to show weak fibrogenic activity and cause pneumoconiosis. The maximum concentration recommended for nitrides of nonmetals is 10 mg/m3 for BN and 4 for AlN or ZrN.
Notes and references
- ^ M. Kawaguchi; Kuroda, Shinya; Muramatsu, Yasuji (2008). "Electronic structure and intercalation chemistry of graphite-like layered material with a composition of BC6N". Journal of Physics and Chemistry of Solids 69 (5–6): 1171. doi:10.1016/j.jpcs.2007.10.076.
- ^ M. S. Silberberg (2009). Chemistry: The Molecular Nature of Matter and Change, Fifth Edition. New York: McGraw-Hill. p. 483.
- ^ T. P. Crane and B. P. Cowan (2000). "Magnetic relaxation properties of helium-3 adsorbed on hexagonal boron nitride". Phys. Rev. B 62 (17): 11359. doi:10.1103/PhysRevB.62.11359.
- ^ R. Zedlitz (1996). "Properties of amorphous boron nitride thin films". Journal of Non-Crystalline Solids 198–200: 403. doi:10.1016/0022-3093(95)00748-2.
- ^ C. H. Henager, Jr. (1993). "Thermal conductivities of thin, sputtered optical films". Applied Optics 32 (1): 91. doi:10.1364/AO.32.000091. PMID 20802666.
- ^ S. Weissmantel (1999). "Microstructure and mechanical properties of pulsed laser deposited boron nitride films". Diamond and Related Materials 8 (2–5): 377. doi:10.1016/S0925-9635(98)00394-X.
- ^ a b c d e f ed.: P. Beiss et al., Authors: G. Leichtfried et al. (2002). "13.5 Properties of diamond and cubic boron nitride". Landolt-Börnstein – Group VIII Advanced Materials and Technologies: Powder Metallurgy Data. Refractory, Hard and Intermetallic Materials. 2A2. Berlin: Springer. pp. 118–139. doi:10.1007/b83029. ISBN 978-3-540-42961-6.
- ^ a b "Ioffe database". http://www.ioffe.ru/SVA/NSM/Semicond/BN/index.html. Retrieved 2009-05-05.
- ^ P. Delhaes (2001). Graphite and Precursors. CRC Press. ISBN 9056992287.
- ^ Z. Pan; Sun, Hong; Zhang, Yi; Chen, Changfeng (2009). "Harder than Diamond: Superior Indentation Strength of Wurtzite BN and Lonsdaleite". Physical Review Letters 102 (5): 055503. Bibcode 2009PhRvL.102e5503P. doi:10.1103/PhysRevLett.102.055503. PMID 19257519.
- ^ a b c d e M. Engler (2007). "Hexagonal Boron Nitride (hBN) – Applications from Metallurgy to Cosmetics". Cfi/Ber. DKG 84: D25. ISSN 0173-9913. http://www.esk.com/uploads/tx_userjspresseveroeff/PR_0712_CFI_12-2007_Hexagonales-BN_e_01.pdf.
- ^ Y. Kubota; Watanabe, K.; Tsuda, O.; Taniguchi, T. (2007). "Deep Ultraviolet Light-Emitting Hexagonal Boron Nitride Synthesized at Atmospheric Pressure". Science 317 (5840): 932. doi:10.1126/science.1144216. PMID 17702939.
- ^ K. Watanabe, T. Taniguchi, H. Kanda (2004). "Direct-bandgap properties and evidence for ultraviolet lasing of hexagonal boron nitride single crystal". Nature Materials 3 (6): 404. doi:10.1038/nmat1134. PMID 15156198.
- ^ T. Taniguchi; Watanabe, K.; Koizumi, S.; Sakaguchi, I.; Sekiguchi, T.; Yamaoka, S. (2002). "Ultraviolet light emission from self-organized p–n domains in cubic boron nitride bulk single crystals grown under high pressure". Appl. Phys. Lett. 81 (22): 4145. doi:10.1063/1.1524295.
- ^ Lloyd H. Dreger; Dadape, V. V.; Margrave, John L. (1962). The Journal of Physical Chemistry 66 (8): 1556. doi:10.1021/j100814a515.
- ^ a b R. H. Wentorf (1957). "Cubic form of boron nitride". J. Chem. Phys. 26 (3): 956. doi:10.1063/1.1731679.
- ^ Here wetting refers to the ability of a molten metal to keep contact with solid BN
- ^ J. H. Lan et al. (2009). "Thermal transport in hexagonal boron nitride nanoribbons". Physical Review B 79 (11): 115401. doi:10.1103/PhysRevB.79.115401.
- ^ Jiuning Hu, Xiulin Ruan and Yong P. Chen (2009). "Thermal Conductivity and Thermal Rectification in Graphene Nanoribbons: A Molecular Dynamics Study". Nano Lett. 9 (7): 2730. doi:10.1021/nl901231s. PMID 19499898.
- ^ Tao Ouyang, Yuanping Chen, Yuee Xie, Kaike Yang, Zhigang Bao and Jianxin Zhong (2010). "Thermal transport in hexagonal boron nitride nanoribbons". Nanotechnology 21 (24): 245701. doi:10.1088/0957-4484/21/24/245701.
- ^ Pradyot Patnaik (2003). Handbook of Inorganic Chemical Compounds. McGraw-Hill. p. 119. ISBN 0070494398. http://books.google.com/?id=Xqj-TTzkvTEC&pg=PA119. Retrieved 2009-06-06.
- ^ a b S. Rudolph (2000). "Boron Nitride: Mineral Review 2000". American Ceramic Society Bulletin 79: 50. http://www.a-m.de/deu/literatur/cb0600.html.
- ^ "Synthesis of Boron Nitride from Oxide Precursors". Archived from the original on December 12, 2007. http://web.archive.org/web/20071212115253/http://hubacek.jp/bn/bn.htm. Retrieved 2009-06-06.
- ^ a b P.B. Mirkarimi; McCarty, K; Medlin, D (1997). "Review of advances in cubic boron nitride film synthesis". Materials Science and Engineering R Reports 21 (2): 47–100. doi:10.1016/S0927-796X(97)00009-0.
- ^ Robert T. Paine, Chaitanya K. Narula (1990). "Synthetic routes to boron nitride". Chem. Rev. 90: 73–91. doi:10.1021/cr00099a004.
- ^ I. Tornieporth-Oetting and T. Klapötke (1990). "Nitrogen Triiodide". Angewandte Chemie International Edition 29 (6): 677–679. doi:10.1002/anie.199006771.
- ^ V. L. Solozhenko; Le Godec, Yann; Klotz, Stefan; Mezouar, Mohamed; Turkevich, Vladimir Z.; Besson, Jean-Michel (2002). "In situ studies of boron nitride crystallization from BN solutions in supercritical N–H fluid at high pressures and temperatures". Phys. Chem. Chem. Phys. 4 (21): 5386. doi:10.1039/b206005a.
- ^ G. L. Doll; Speck, J. S.; Dresselhaus, G.; Dresselhaus, M. S.; Nakamura, K.; Tanuma, S.-I. (1989). "Intercalation of hexagonal boron nitride with potassium". J. Appl. Phys. 66 (6): 2554. doi:10.1063/1.344219.
- ^ Bai-Qing Dai and Gui-Ling Zhang (2003). "A DFT study of hBN compared with graphite in forming alkali metal intercalation compounds". Materials Chemistry and Physics 78 (2): 304. doi:10.1016/S0254-0584(02)00205-5.
- ^ a b L. Vel; Demazeau, G; Etourneau, J (1991). "Cubic boron nitride: synthesis, physicochemical properties and applications". Materials Science and Engineering: B 10 (2): 149. doi:10.1016/0921-5107(91)90121-B.
- ^ O. Fukunaga (2002). "Science and technology in the recent development of boron nitride materials". J. Phys.: Condens. Matter 14 (44): 10979. doi:10.1088/0953-8984/14/44/413.
- ^ T. Komatsu; Samedima, Miho; Awano, Ternyuki; Kakadate, Yozo; Fujiwara, Syuzo (1999). "Creation of superhard B–C–N heterodiamond using an advanced shock wave compression technology". Journal of Materials Processing Technology 85: 69. doi:10.1016/S0924-0136(98)00263-5.
- ^ T. Soma; Sawaoka, A; Saito, S (1974). "Characterization of wurtzite type boron nitride synthesized by shock compression". Materials Research Bulletin 9 (6): 755. doi:10.1016/0025-5408(74)90110-X.
- ^ a b Jochen Greim, Karl A. Schwetz (2005). Boron Carbide, Boron Nitride, and Metal Borides, in Ullmann's Encyclopedia of Industrial Chemistry. Wiley-VCH: Weinheim. doi:10.1002/14356007.a04_295.pub2.
- ^ R.F. Davis (1991). "III-V nitrides for electronic and optoelectronic applications". Proceedings of the IEEE 79 (5): 702–712. doi:10.1109/5.90133.
- ^ L.B. Schein (1988). Electrophotography and Development Physics, Springer Series in Electrophysics. 14. Springer-Verlag, Berlin.
- ^ Charles A. Harper (2001). Handbook of ceramics, glasses and diamonds. McGraw-Hill. ISBN 007026712X.
- ^ Todd, Robert H.; Allen, Dell K.; Alting, Leo (1994). Manufacturing Processes Reference Guide. Industrial Press Inc.. pp. 43–48. ISBN 0-8311-3049-0. http://books.google.com/?id=6x1smAf_PAcC.
- ^ M. A. El Khakani and M. Chaker (1993). "Physical properties of the x-ray membrane materials". J. Vac. Sci. Technol. B 11 (6): 2930. doi:10.1116/1.586563.
- ^ W. Schmolla (1985). "Positive drift effect of BN-InP enhancement n-channel MISFET". International Journal of Electronics 58: 35. doi:10.1080/00207218508939000.
- ^ T. S. Bartnitskaya; Ostrovskaya, N. F.; Ul'yanova, T. M.; Fenochka, B. V. (1999). "Preparation of boron nitride fibers with the use of hydrated cellulose. I. Decomposition of hydrated cellulose impregnated with boron-containing compounds". Powder Metallurgy and Metal Ceramics 38 (3–4): 152. doi:10.1007/BF02676041.
- ^ a b c M. Corso; Auwärter, W; Muntwiler, M; Tamai, A; Greber, T; Osterwalder, J (2004). "Boron Nitride Nanomesh". Science 303 (5655): 217–220. doi:10.1126/science.1091979. PMID 14716010.
- ^ a b A. Goriachko; He, Y; Knapp, Marcus; Over, Herbert; Corso, Martina; Brugger, Thomas; Berner, Simon; Osterwalder, Juerg et al. (2007). "Self-assembly of a hexagonal boron nitride nanomesh on Ru(0001)". Langmuir Lett. 23 (6): 2928–2931. doi:10.1021/la062990t. PMID 17286422.
- ^ O. Bunk; Corso, M; Martoccia, D; Herger, R; Willmott, P; Patterson, B; Osterwalder, J; Vanderveen, J et al. (2007). "Surface X-ray diffraction study of boron-nitride nanomesh in air". Surf. Sci. 601 (2): L7–L10. doi:10.1016/j.susc.2006.11.018.
- ^ a b S. Berner; Corso, Martina; Widmer, Roland; Groening, Oliver; Laskowski, Robert; Blaha, Peter; Schwarz, Karlheinz; Goriachko, Andrii et al. (2007). "Boron Nitride Nanomesh: Functionality from a Corrugated Monolayer". Angew. Chem. Int. Ed. 46 (27): 5115–5119. doi:10.1002/anie.200700234. PMID 17538919.
- ^ R. Widmer; Berner, S; Groning, O; Brugger, T; Osterwalder, J; Greber, T (2007). "Electrolytic in situ STM investigation of h-BN-Nanomesh". Electrochem. Comm. 9 (10): 2484–2488. doi:10.1016/j.elecom.2007.07.019.
- ^ "The discovery of the nanomesh for everyone". http://www.nanomesh.ch/history.php. Retrieved 2009-06-06.
- ^ Rubio, Angel; Corkill, Jennifer; Cohen, Marvin (1994). "Theory of graphitic boron nitride nanotubes". Physical Review B 49 (7): 5081. doi:10.1103/PhysRevB.49.5081.
- ^ a b Chopra, N. G.; Luyken, R. J.; Cherrey, K.; Crespi, V. H.; Cohen, M. L.; Louie, S. G.; Zettl, A. (1995). "Boron Nitride Nanotubes". Science 269 (5226): 966. doi:10.1126/science.269.5226.966. PMID 17807732.
- ^ Blase, X; Rubio, A; Louie, S. G; Cohen, M. L (1994). "Stability and Band Gap Constancy of Boron Nitride Nanotubes". Europhysics Letters (EPL) 28 (5): 335. doi:10.1209/0295-5075/28/5/007.
- ^ Han, Wei-Qiang; Mickelson, W.; Cumings, John; Zettl, A. (2002). "Transformation of B[sub xC[sub y]N[sub z] nanotubes to pure BN nanotubes"]. Applied Physics Letters 81 (6): 1110. doi:10.1063/1.1498494. http://www.glue.umd.edu/~cumings/PDF%20Publications/15.APL81han.pdf.
- ^ D. Golberg, Y. Bando, C.C. Tang, C.Y. Zhi (2007). "Boron nitride nanotubes". Adv. Mater. 19 (18): 2413. doi:10.1002/adma.200700179.
- ^ Cumings, J (2000). "Mass-production of boron nitride double-wall nanotubes and nanococoons". Chemical Physics Letters 316 (3–4): 211. Bibcode 2000CPL...316..211C. doi:10.1016/S0009-2614(99)01277-4.
- ^ Golberg, D.; Bando, Y.; Eremets, M.; Takemura, K.; Kurashima, K.; Yusa, H. (1996). "Nanotubes in boron nitride laser heated at high pressure". Applied Physics Letters 69 (14): 2045. doi:10.1063/1.116874.
- ^ Yu, D. P.; Sun, X. S.; Lee, C. S.; Bello, I.; Lee, S. T.; Gu, H. D.; Leung, K. M.; Zhou, G. W. et al. (1998). "Synthesis of boron nitride nanotubes by means of excimer laser ablation at high temperature". Applied Physics Letters 72 (16): 1966. doi:10.1063/1.121236.
- ^ Zhi, C; Bando, Y; Tan, C; Golberg, D (2005). "Effective precursor for high yield synthesis of pure BN nanotubes". Solid State Communications 135: 67. doi:10.1016/j.ssc.2005.03.062.
- ^ a b H. Chen; Zhang, Hongzhou; Fu, Lan; Chen, Ying; Williams, James S.; Yu, Chao; Yu, Dapeng (2008). "Nano Au-decorated boron nitride nanotubes: Conductance modification and field-emission enhancement". Appl. Phys. Lett. 92 (24): 243105. doi:10.1063/1.2943653. http://wwwrsphysse.anu.edu.au/nanotube/pdf/aubnntapl08.pdf.
- ^ a b H. Chen; Chen, Y.; Li, C. P.; Zhang, H.; Williams, J. S.; Liu, Y.; Liu, Z.; Ringer, S. P. (2007). "Eu-doped Boron Nitride Nanotubes as a Nanometer-Sized Visible-Light Source". Advanced Materials 19 (14): 1845. doi:10.1002/adma.200700493. http://wwwrsphysse.anu.edu.au/nanotube/pdf/Eu-BNNTs.pdf.
- ^ Y. Chen; Fu, L.; Chen, Y.; Zou, J.; Li, J.; Duan, W. H. (2008). "Au doped BN nanotubes with tunable conductivity". Nano 2 (06): 367. doi:10.1142/S1793292007000702.
- ^ J. Yu; Chen, Y.; Elliman, R. G.; Petravic, M. (2006). "Isotopically Enriched 10BN Nanotubes". Advanced Materials 18 (16): 2157. doi:10.1002/adma.200600231. http://www.rsphysse.anu.edu.au/nanotube/pdf/B10Nnanotubes.pdf.
- ^ S. M. Lee (1992). Handbook of Composite Reinforcements. John Wiley and Sons. ISBN 0471188611.
- Synthesis and functionalization of BN nanotubes
- National Pollutant Inventory: Boron and Compounds
- Materials Safety Data Sheet at University of Oxford
Wikimedia Foundation. 2010.
Look at other dictionaries:
boron nitride — n. a white, powdery compound, BN, of boron and nitrogen, with high electrical resistance: it can be compressed, under a million pounds of pressure, to form Borazon … English World dictionary
boron nitride — Chem. a white powder, BN, formed by heating boron in nitrogen. In its ordinary form, it has a structure of stacked layers of hexagonal rings, very similar to that of graphite, and is used as a refractory electrical insulator. Cf. Borazon. * * * ▪ … Universalium
boron nitride — noun : any binary compound of boron and nitrogen; especially : a fluffy white crystalline powder BN made in various ways (as by the reaction of ammonia and fused boric oxide) and used chiefly as a lubricant and electric insulator * * * Chem. a… … Useful english dictionary
boron nitride — boro nitridas statusas T sritis chemija formulė BN atitikmenys: angl. boron nitride rus. бор азотистый; бора нитрид … Chemijos terminų aiškinamasis žodynas
boron nitride — noun A binary compound of boron and nitrogen, of empirical formula BN; exists in forms analagous to the allotropes of carbon, many of which are inorganic polymers … Wiktionary
boron nitride — Смотри нитрид бора … Энциклопедический словарь по металлургии
boron-nitride diffusion source — boro nitrido difuzijos šaltinis statusas T sritis radioelektronika atitikmenys: angl. boron nitride diffusion source vok. Bornitriddifusionsquelle, f rus. источник диффузии на основе нитрида бора, m pranc. nitrure de bore en source de diffusion,… … Radioelektronikos terminų žodynas
boron nitride pellicle — boro nitrido plėvelė statusas T sritis radioelektronika atitikmenys: angl. boron nitride pellicle vok. Bornitridfilm, m rus. плёнка нитрида бора, f pranc. pellicule de nitrure de bore, f … Radioelektronikos terminų žodynas
Boron — (pronEng|ˈbɔərɒn) is a chemical element with atomic number 5 and the chemical symbol B. Boron is a trivalent nonmetallic element which occurs abundantly in the evaporite ores borax and ulexite. Boron is never found as a free element on… … Wikipedia
nitride — /nuy truyd, trid/, n. Chem. a compound, containing two elements only, of which the more electronegative one is nitrogen. [1840 50; NITR + IDE] * * * ▪ chemical compound Introduction any of a class of chemical compounds in which nitrogen is… … Universalium